The thermal conductivity of a material is a measure of its ability to conduct heat. It is commonly denoted by , , or .
Heat transfer occurs at a lower rate in materials of low thermal conductivity than in materials of high thermal conductivity. For instance, metals typically have high thermal conductivity and are very efficient at conducting heat, while the opposite is true for insulating materials like Styrofoam. Correspondingly, materials of high thermal conductivity are widely used in heat sink applications, and materials of low thermal conductivity are used as thermal insulation. The reciprocal of thermal conductivity is called thermal resistivity.
The defining equation for thermal conductivity is , where is the heat flux, is the thermal conductivity, and is the temperature gradient. This is known as Fourier's Law for heat conduction. Although commonly expressed as a scalar, the most general form of thermal conductivity is a second-rank tensor. However, the tensorial description only becomes necessary in materials which are anisotropic.
Consider a solid material placed between two environments of different temperatures. Let be the temperature at and be the temperature at , and suppose . A possible realization of this scenario is a building on a cold winter day: the solid material in this case would be the building wall, separating the cold outdoor environment from the warm indoor environment.
According to the second law of thermodynamics, heat will flow from the hot environment to the cold one in an attempt to equalize the temperature difference. This is quantified in terms of a heat flux , which gives the rate, per unit area, at which heat flows in a given direction (in this case minus x-direction). In many materials, is observed to be directly proportional to the temperature difference and inversely proportional to the separation distance :^{[1]}
The constant of proportionality is the thermal conductivity; it is a physical property of the material. In the present scenario, since heat flows in the minus x-direction and is negative, which in turn means that . In general, is always defined to be positive. The same definition of can also be extended to gases and liquids, provided other modes of energy transport, such as convection and radiation, are eliminated.
For simplicity, we have assumed here that the does not vary significantly as temperature is varied from to . Cases in which the temperature variation of is non-negligible must be addressed using the more general definition of discussed below.
Thermal conduction is defined as the transport of energy due to random molecular motion across a temperature gradient. It is distinguished from energy transport by convection and molecular work in that it does not involve macroscopic flows or work-performing internal stresses.
Energy flow due to thermal conduction is classified as heat and is quantified by the vector , which gives the heat flux at position and time . According to the second law of thermodynamics, heat flows from high to low temperature. Hence, it is reasonable to postulate that is proportional to the gradient of the temperature field , i.e.
where the constant of proportionality, , is the thermal conductivity. This is called Fourier's law of heat conduction. In actuality, it is not a law but a definition of thermal conductivity in terms of the independent physical quantities and .^{[2]}^{[3]} As such, its usefulness depends on the ability to determine for a given material under given conditions. The constant itself usually depends on and thereby implicitly on space and time. An explicit space and time dependence could also occur if the material is inhomogeneous or changing with time.^{[4]}
In some solids, thermal conduction is anisotropic, i.e. the heat flux is not always parallel to the temperature gradient. To account for such behavior, a tensorial form of Fourier's law must be used:
where is symmetric, second-rank tensor called the thermal conductivity tensor.^{[5]}
An implicit assumption in the above description is the presence of local thermodynamic equilibrium, which allows one to define a temperature field .
In engineering practice, it is common to work in terms of quantities which are derivative to thermal conductivity and implicitly take into account design-specific features such as component dimensions.
For instance, thermal conductance is defined as the quantity of heat that passes in unit time through a plate of particular area and thickness when its opposite faces differ in temperature by one kelvin. For a plate of thermal conductivity , area and thickness , the conductance is , measured in W?K^{-1}.^{[6]} The relationship between thermal conductivity and conductance is analogous to the relationship between electrical conductivity and electrical conductance.
Thermal resistance is the inverse of thermal conductance.^{[6]} It is a convenient measure to use in multicomponent design since thermal resistances are additive when occurring in series.^{[7]}
There is also a measure known as the heat transfer coefficient: the quantity of heat that passes per unit time through a unit area of a plate of particular thickness when its opposite faces differ in temperature by one kelvin.^{[8]} In ASTM C168-15, this area-independent quantity is referred to as the "thermal conductance".^{[9]} The reciprocal of the heat transfer coefficient is thermal insulance. In summary, for a plate of thermal conductivity , area and thickness , we have
The heat transfer coefficient is also known as thermal admittance in the sense that the material may be seen as admitting heat to flow.^{[]}
An additional term, thermal transmittance, quantifies the thermal conductance of a structure along with heat transfer due to convection and radiation.^{[]} It is measured in the same units as thermal conductance and is sometimes known as the composite thermal conductance. The term U-value is also used.
Finally, thermal diffusivity combines thermal conductivity with density and specific heat:^{[10]}
As such, it quantifies the thermal inertia of a material, i.e. the relative difficulty in heating a material to a given temperature using heat sources applied at the boundary.^{[11]}
In the International System of Units (SI), thermal conductivity is measured in watts per meter-kelvin (W/(m?K)). Some papers report in watts per centimeter-kelvin (W/(cm?K)).
In imperial units, thermal conductivity is measured in BTU/(h?ft?°F).^{[note 1]}^{[12]}
The dimension of thermal conductivity is M^{1}L^{1}T^{-3}?^{-1}, expressed in terms of the dimensions mass (M), length (L), time (T), and temperature (?).
Other units which are closely related to the thermal conductivity are in common use in the construction and textile industries. The construction industry makes use of measures such as the R-value (resistance) and the U-value (transmittance or conductance). Although related to the thermal conductivity of a material used in an insulation product or assembly, R- and U-values are measured per unit area, and depend on the specified thickness of the product or assembly.^{[note 2]}
Likewise the textile industry has several units including the tog and the clo which express thermal resistance of a material in a way analogous to the R-values used in the construction industry.
There are several ways to measure thermal conductivity; each is suitable for a limited range of materials. Broadly speaking, there are two categories of measurement techniques: steady-state and transient. Steady-state techniques infer the thermal conductivity from measurements on the state of a material once a steady-state temperature profile has been reached, whereas transient techniques operate on the instantaneous state of a system during the approach to steady state. Lacking an explicit time component, steady-state techniques do not require complicated signal analysis (steady state implies constant signals). The disadvantage is that a well-engineered experimental setup is usually needed, and the time required to reach steady state precludes rapid measurement.
In comparison with solid materials, the thermal properties of fluids are more difficult to study experimentally. This is because in addition to thermal conduction, convective and radiative energy transport are usually present unless measures are taken to limit these processes. The formation of an insulating boundary layer can also result in an apparent reduction in the thermal conductivity.^{[13]}^{[14]}
The thermal conductivities of common substances span at least four orders of magnitude. Gases generally have low thermal conductivity, and pure metals have high thermal conductivity. For example, under standard conditions the thermal conductivity of copper is over times that of air.
Of all materials, allotropes of carbon, such as graphite and diamond, are usually credited with having the highest thermal conductivities at room temperature.^{[15]} The thermal conductivity of natural diamond at room temperature is several times higher than that of a highly conductive metal such as copper (although the precise value varies depending on the diamond type).^{[16]}
Thermal conductivities of selected substances are tabulated here; an expanded list can be found in the list of thermal conductivities. These values should be considered approximate due to the uncertainties related to material definitions.
Substance | Thermal conductivity (W·m^{-1}·K^{-1}) | Temperature (°C) |
---|---|---|
Air^{[17]} | 0.026 | 25 |
Styrofoam^{[18]} | 0.033 | 25 |
Water^{[19]} | 0.6089 | 26.85 |
Concrete^{[19]} | 0.92 | - |
Copper^{[19]} | 384.1 | 18.05 |
Natural diamond^{[16]} | 895-1350 | 26.85 |
The effect of temperature on thermal conductivity is different for metals and nonmetals. In metals, heat conductivity is primarily due to free electrons. Following the Wiedemann-Franz law, thermal conductivity of metals is approximately proportional to the absolute temperature (in kelvins) times electrical conductivity. In pure metals the electrical conductivity decreases with increasing temperature and thus the product of the two, the thermal conductivity, stays approximately constant. However, as temperatures approach absolute zero, the thermal conductivity decreases sharply.^{[20]} In alloys the change in electrical conductivity is usually smaller and thus thermal conductivity increases with temperature, often proportionally to temperature. Many pure metals have a peak thermal conductivity between 2 K and 10 K.
On the other hand, heat conductivity in nonmetals is mainly due to lattice vibrations (phonons). Except for high-quality crystals at low temperatures, the phonon mean free path is not reduced significantly at higher temperatures. Thus, the thermal conductivity of nonmetals is approximately constant at high temperatures. At low temperatures well below the Debye temperature, thermal conductivity decreases, as does the heat capacity, due to carrier scattering from defects at very low temperatures.^{[20]}
When a material undergoes a phase change (e.g. from solid to liquid), the thermal conductivity may change abruptly. For instance, when ice melts to form liquid water at 0 °C, the thermal conductivity changes from 2.18 W/(m?K) to 0.56 W/(m?K).^{[21]}
Even more dramatically, the thermal conductivity of a fluid diverges in the vicinity of the vapor-liquid critical point.^{[22]}
Some substances, such as non-cubic crystals, can exhibit different thermal conductivities along different crystal axes, due to differences in phonon coupling along a given crystal axis. Sapphire is a notable example of variable thermal conductivity based on orientation and temperature, with 35 W/(m?K) along the c axis and 32 W/(m?K) along the a axis.^{[23]}Wood generally conducts better along the grain than across it. Other examples of materials where the thermal conductivity varies with direction are metals that have undergone heavy cold pressing, laminated materials, cables, the materials used for the Space Shuttle thermal protection system, and fiber-reinforced composite structures.^{[24]}
When anisotropy is present, the direction of heat flow may not be exactly the same as the direction of the thermal gradient.
In metals, thermal conductivity approximately tracks electrical conductivity according to the Wiedemann-Franz law, as freely moving valence electrons transfer not only electric current but also heat energy. However, the general correlation between electrical and thermal conductance does not hold for other materials, due to the increased importance of phonon carriers for heat in non-metals. Highly electrically conductive silver is less thermally conductive than diamond, which is an electrical insulator but conducts heat via phonons due to its orderly array of atoms.
The influence of magnetic fields on thermal conductivity is known as the thermal Hall effect or Righi-Leduc effect.
Air and other gases are generally good insulators, in the absence of convection. Therefore, many insulating materials function simply by having a large number of gas-filled pockets which obstruct heat conduction pathways. Examples of these include expanded and extruded polystyrene (popularly referred to as "styrofoam") and silica aerogel, as well as warm clothes. Natural, biological insulators such as fur and feathers achieve similar effects by trapping air in pores, pockets or voids, thus dramatically inhibiting convection of air or water near an animal's skin.
Low density gases, such as hydrogen and helium typically have high thermal conductivity. Dense gases such as xenon and dichlorodifluoromethane have low thermal conductivity. An exception, sulfur hexafluoride, a dense gas, has a relatively high thermal conductivity due to its high heat capacity. Argon and krypton, gases denser than air, are often used in insulated glazing (double paned windows) to improve their insulation characteristics.
The thermal conductivity through bulk materials in porous or granular form is governed by the type of gas in the gaseous phase, and its pressure.^{[25]} At lower pressures, the thermal conductivity of a gaseous phase is reduced, with this behaviour governed by the Knudsen number, defined as , where is the mean free path of gas molecules and is the typical gap size of the space filled by the gas. In a granular material corresponds to the characteristic size of the gaseous phase in the pores or intergranular spaces.^{[25]}
The thermal conductivity of a crystal can depend strongly on isotopic purity, assuming other lattice defects are negligible. A notable example is diamond: at a temperature of around 100 K the thermal conductivity increases from 10,000 W·m^{-1}·K^{-1} for natural type IIa diamond (98.9% ^{12}C), to 41,000 for 99.9% enriched synthetic diamond. A value of 200,000 is predicted for 99.999% ^{12}C at 80 K, assuming an otherwise pure crystal.^{[26]}
The atomic mechanisms of thermal conduction vary among different materials, and in general depend on details of the microscopic structure and atomic interactions. As such, thermal conductivity is difficult to predict from first-principles. Any expressions for thermal conductivity which are exact and general, e.g. the Green-Kubo relations, are difficult to apply in practice, typically consisting of averages over multiparticle correlation functions.^{[27]} A notable exception is a dilute gas, for which a well-developed theory exists expressing thermal conductivity accurately and explicitly in terms of molecular parameters.
In a gas, thermal conduction is mediated by discrete molecular collisions. In a simplified picture of a solid, thermal conduction occurs by two mechanisms: 1) the migration of free electrons and 2) lattice vibrations (phonons). The first mechanism dominates in pure metals and the second in non-metallic solids. In liquids, by contrast, the precise microscopic mechanisms of thermal conduction are poorly understood.^{[28]}
In a simplified model of a dilute monatomic gas, molecules are modeled as rigid spheres which are in constant motion, colliding elastically with each other and with the walls of their container. Consider such a gas at temperature and with density , specific heat and molecular mass . Under these assumptions, an elementary calculation yields for the thermal conductivity
where is a numerical constant of order , is the Boltzmann constant, and is the mean free path, which measures the average distance a molecule travels between collisions.^{[29]} Since is inversely proportional to density, this equation predicts that thermal conductivity is independent of density for fixed temperature. The explanation is that increasing density increases the number of molecules which carry energy but decreases the average distance a molecule can travel before transferring its energy to a different molecule: these two effects cancel out. For most gases, this prediction agrees well with experiments at pressures up to about 10 atmospheres.^{[30]} On the other hand, experiments show a more rapid increase with temperature than (here is independent of ). This failure of the elementary theory can be traced to the oversimplified "elastic sphere" model, and in particular to the fact that the interparticle attractions, present in all real-world gases, are ignored.
To incorporate more complex interparticle interactions, a systematic approach is necessary. One such approach is provided by Chapman-Enskog theory, which derives explicit expressions for thermal conductivity starting from the Boltzmann equation. The Boltzmann equation, in turn, provides a statistical description of a dilute gas for generic interparticle interactions. For a monatomic gas, expressions for derived in this way take the form
where is an effective particle diameter and is a function of temperature whose explicit form depends on the interparticle interaction law.^{[31]}^{[32]} For rigid elastic spheres, is independent of and very close to . More complex interaction laws introduce a weak temperature dependence. The precise nature of the dependence is not always easy to discern, however, as is defined as a multi-dimensional integral which may not be expressible in terms of elementary functions. An alternate, equivalent way to present the result is in terms of the gas viscosity , which can also be calculated in the Chapman-Enskog approach:
where is a numerical factor which in general depends on the molecular model. For smooth spherically symmetric molecules, however, is very close to , not deviating by more than for a variety of interparticle force laws.^{[33]} Since , , and are each well-defined physical quantities which can be measured independent of each other, this expression provides a convenient test of the theory. For monatomic gases, such as the noble gases, the agreement with experiment is fairly good.^{[34]}
For gases whose molecules are not spherically symmetric, the expression still holds. In contrast with spherically symmetric molecules, however, varies significantly depending on the particular form of the interparticle interactions: this is a result of the energy exchanges between the internal and translational degrees of freedom of the molecules. An explicit treatment of this effect is difficult in the Chapman-Enskog approach. Alternately, the approximate expression was suggested by Eucken, where is the heat capacity ratio of the gas.^{[33]}^{[35]}
The entirety of this section assumes the mean free path is small compared with macroscopic (system) dimensions. In extremely dilute gases this assumption fails, and thermal conduction is described instead by an apparent thermal conductivity which decreases with density. Ultimately, as the density goes to the system approaches a vacuum, and thermal conduction ceases entirely. For this reason a vacuum is an effective insulator.
The exact mechanisms of thermal conduction are poorly understood in liquids: there is no molecular picture which is both simple and accurate. An example of a simple but very rough theory is that of Bridgman, in which a liquid is ascribed a local molecular structure similar to that of a solid, i.e. with molecules located approximately on a lattice. Elementary calculations then lead to the expression
where is the Avogadro constant, is the volume of a mole of liquid, and is the speed of sound in the liquid. This is commonly called Bridgman's equation.^{[36]}
For metals at low temperatures the heat is carried mainly by the free electrons. In this case the mean velocity is the Fermi velocity which is temperature independent. The mean free path is determined by the impurities and the crystal imperfections which are temperature independent as well. So the only temperature-dependent quantity is the heat capacity c, which, in this case, is proportional to T. So
with k_{0} a constant. For pure metals such as copper, silver, etc. k_{0} is large, so the thermal conductivity is high. At higher temperatures the mean free path is limited by the phonons, so the thermal conductivity tends to decrease with temperature. In alloys the density of the impurities is very high, so l and, consequently k, are small. Therefore, alloys, such as stainless steel, can be used for thermal insulation.
This section may be too technical for most readers to understand.January 2019) (Learn how and when to remove this template message) ( |
This article relies too much on references to primary sources. (February 2021) (Learn how and when to remove this template message) |
Heat transport in both amorphous and crystalline dielectric solids is by way of elastic vibrations of the lattice (i.e., phonons). This transport mechanism is theorized to be limited by the elastic scattering of acoustic phonons at lattice defects. This has been confirmed by the experiments of Chang and Jones on commercial glasses and glass ceramics, where the mean free paths were found to be limited by "internal boundary scattering" to length scales of 10^{-2} cm to 10^{-3} cm.^{[37]}^{[38]}
The phonon mean free path has been associated directly with the effective relaxation length for processes without directional correlation. If V_{g} is the group velocity of a phonon wave packet, then the relaxation length is defined as:
where t is the characteristic relaxation time. Since longitudinal waves have a much greater phase velocity than transverse waves,^{[39]}V_{long} is much greater than V_{trans}, and the relaxation length or mean free path of longitudinal phonons will be much greater. Thus, thermal conductivity will be largely determined by the speed of longitudinal phonons.^{[37]}^{[40]}
Regarding the dependence of wave velocity on wavelength or frequency (dispersion), low-frequency phonons of long wavelength will be limited in relaxation length by elastic Rayleigh scattering. This type of light scattering from small particles is proportional to the fourth power of the frequency. For higher frequencies, the power of the frequency will decrease until at highest frequencies scattering is almost frequency independent. Similar arguments were subsequently generalized to many glass forming substances using Brillouin scattering.^{[41]}^{[42]}^{[43]}^{[44]}
Phonons in the acoustical branch dominate the phonon heat conduction as they have greater energy dispersion and therefore a greater distribution of phonon velocities. Additional optical modes could also be caused by the presence of internal structure (i.e., charge or mass) at a lattice point; it is implied that the group velocity of these modes is low and therefore their contribution to the lattice thermal conductivity ?_{L} (_{L}) is small.^{[45]}
Each phonon mode can be split into one longitudinal and two transverse polarization branches. By extrapolating the phenomenology of lattice points to the unit cells it is seen that the total number of degrees of freedom is 3pq when p is the number of primitive cells with q atoms/unit cell. From these only 3p are associated with the acoustic modes, the remaining 3p(q - 1) are accommodated through the optical branches. This implies that structures with larger p and q contain a greater number of optical modes and a reduced ?_{L}.
From these ideas, it can be concluded that increasing crystal complexity, which is described by a complexity factor CF (defined as the number of atoms/primitive unit cell), decreases ?_{L}.^{[46]}^{[failed verification]} This was done by assuming that the relaxation time ? decreases with increasing number of atoms in the unit cell and then scaling the parameters of the expression for thermal conductivity in high temperatures accordingly.^{[45]}
Describing anharmonic effects is complicated because an exact treatment as in the harmonic case is not possible, and phonons are no longer exact eigensolutions to the equations of motion. Even if the state of motion of the crystal could be described with a plane wave at a particular time, its accuracy would deteriorate progressively with time. Time development would have to be described by introducing a spectrum of other phonons, which is known as the phonon decay. The two most important anharmonic effects are the thermal expansion and the phonon thermal conductivity.
Only when the phonon number
where v is the energy transport velocity of phonons. Only two mechanisms exist that can cause time variation of n> in a particular region. The number of phonons that diffuse into the region from neighboring regions differs from those that diffuse out, or phonons decay inside the same region into other phonons. A special form of the Boltzmann equation
states this. When steady state conditions are assumed the total time derivate of phonon number is zero, because the temperature is constant in time and therefore the phonon number stays also constant. Time variation due to phonon decay is described with a relaxation time (?) approximation
which states that the more the phonon number deviates from its equilibrium value, the more its time variation increases. At steady state conditions and local thermal equilibrium are assumed we get the following equation
Using the relaxation time approximation for the Boltzmann equation and assuming steady-state conditions, the phonon thermal conductivity ?_{L} can be determined. The temperature dependence for ?_{L} originates from the variety of processes, whose significance for ?_{L} depends on the temperature range of interest. Mean free path is one factor that determines the temperature dependence for ?_{L}, as stated in the following equation
where ? is the mean free path for phonon and denotes the heat capacity. This equation is a result of combining the four previous equations with each other and knowing that for cubic or isotropic systems and .^{[47]}
At low temperatures (< 10 K) the anharmonic interaction does not influence the mean free path and therefore, the thermal resistivity is determined only from processes for which q-conservation does not hold. These processes include the scattering of phonons by crystal defects, or the scattering from the surface of the crystal in case of high quality single crystal. Therefore, thermal conductance depends on the external dimensions of the crystal and the quality of the surface. Thus, temperature dependence of ?_{L} is determined by the specific heat and is therefore proportional to T^{3}.^{[47]}
Phonon quasimomentum is defined as ?q and differs from normal momentum because it is only defined within an arbitrary reciprocal lattice vector. At higher temperatures (10 K < T < ?), the conservation of energy and quasimomentum , where q_{1} is wave vector of the incident phonon and q_{2}, q_{3} are wave vectors of the resultant phonons, may also involve a reciprocal lattice vector G complicating the energy transport process. These processes can also reverse the direction of energy transport.
Therefore, these processes are also known as Umklapp (U) processes and can only occur when phonons with sufficiently large q-vectors are excited, because unless the sum of q_{2} and q_{3} points outside of the Brillouin zone the momentum is conserved and the process is normal scattering (N-process). The probability of a phonon to have energy E is given by the Boltzmann distribution . To U-process to occur the decaying phonon to have a wave vector q_{1} that is roughly half of the diameter of the Brillouin zone, because otherwise quasimomentum would not be conserved.
Therefore, these phonons have to possess energy of , which is a significant fraction of Debye energy that is needed to generate new phonons. The probability for this is proportional to , with . Temperature dependence of the mean free path has an exponential form . The presence of the reciprocal lattice wave vector implies a net phonon backscattering and a resistance to phonon and thermal transport resulting finite ?_{L},^{[45]} as it means that momentum is not conserved. Only momentum non-conserving processes can cause thermal resistance.^{[47]}
At high temperatures (T > ?), the mean free path and therefore ?_{L} has a temperature dependence T^{-1}, to which one arrives from formula by making the following approximation ^{[clarification needed]} and writing . This dependency is known as Eucken's law and originates from the temperature dependency of the probability for the U-process to occur.^{[45]}^{[47]}
Thermal conductivity is usually described by the Boltzmann equation with the relaxation time approximation in which phonon scattering is a limiting factor. Another approach is to use analytic models or molecular dynamics or Monte Carlo based methods to describe thermal conductivity in solids.
Short wavelength phonons are strongly scattered by impurity atoms if an alloyed phase is present, but mid and long wavelength phonons are less affected. Mid and long wavelength phonons carry significant fraction of heat, so to further reduce lattice thermal conductivity one has to introduce structures to scatter these phonons. This is achieved by introducing interface scattering mechanism, which requires structures whose characteristic length is longer than that of impurity atom. Some possible ways to realize these interfaces are nanocomposites and embedded nanoparticles or structures.
This section does not cite any sources. (August 2018) (Learn how and when to remove this template message) |
Specific thermal conductivity is a materials property used to compare the heat-transfer ability of different materials (i.e., an intensive property). Absolute thermal conductivity, in contrast, is a component property used to compare the heat-transfer ability of different components (i.e., an extensive property). Components, as opposed to materials, take into account size and shape, including basic properties such as thickness and area, instead of just material type. In this way, thermal-transfer ability of components of the same physical dimensions, but made of different materials, may be compared and contrasted, or components of the same material, but with different physical dimensions, may be compared and contrasted.
In component datasheets and tables, since actual, physical components with distinct physical dimensions and characteristics are under consideration, thermal resistance is frequently given in absolute units of or , since the two are equivalent. However, thermal conductivity, which is its reciprocal, is frequently given in specific units of . It is therefore often necessary to convert between absolute and specific units, by also taking a component's physical dimensions into consideration, in order to correlate the two using information provided, or to convert tabulated values of specific thermal conductivity into absolute thermal resistance values for use in thermal resistance calculations. This is particularly useful, for example, when calculating the maximum power a component can dissipate as heat, as demonstrated in the example calculation here.
"Thermal conductivity ? is defined as ability of material to transmit heat and it is measured in watts per square metre of surface area for a temperature gradient of 1 K per unit thickness of 1 m".^{[48]} Therefore, specific thermal conductivity is calculated as:
where:
= temperature difference (K, or °C) = 1 K during measurement
Absolute thermal conductivity, on the other hand, has units of or , and can be expressed as
where = absolute thermal conductivity (W/K, or W/°C).
Substituting for into the first equation yields the equation which converts from absolute thermal conductivity to specific thermal conductivity:
Solving for , we get the equation which converts from specific thermal conductivity to absolute thermal conductivity:
Again, since thermal conductivity and resistivity are reciprocals of each other, it follows that the equation to convert specific thermal conductivity to absolute thermal resistance is:
The thermal conductivity of T-Global L37-3F thermal conductive pad is given as 1.4 W/(mK). Looking at the datasheet and assuming a thickness of 0.3 mm (0.0003 m) and a surface area large enough to cover the back of a TO-220 package (approx. 14.33 mm x 9.96 mm [0.01433 m x 0.00996 m]),^{[49]} the absolute thermal resistance of this size and type of thermal pad is:
This value fits within the normal values for thermal resistance between a device case and a heat sink: "the contact between the device case and heat sink may have a thermal resistance of between 0.5 up to 1.7 °C/W, depending on the case size, and use of grease or insulating mica washer".^{[50]}
In an isotropic medium, the thermal conductivity is the parameter k in the Fourier expression for the heat flux
where is the heat flux (amount of heat flowing per second and per unit area) and the temperature gradient. The sign in the expression is chosen so that always k > 0 as heat always flows from a high temperature to a low temperature. This is a direct consequence of the second law of thermodynamics.
In the one-dimensional case, q = H/A with H the amount of heat flowing per second through a surface with area A and the temperature gradient is dT/dx so
In case of a thermally insulated bar (except at the ends) in the steady state, H is constant. If A is constant as well the expression can be integrated with the result
where T_{H} and T_{L} are the temperatures at the hot end and the cold end respectively, and L is the length of the bar. It is convenient to introduce the thermal-conductivity integral
The heat flow rate is then given by
If the temperature difference is small, k can be taken as constant. In that case